advertisement

PA223 UNIT 4 REVISION LECTURE SEMICONDUCTORS All notes/overheads etc. from Unit 4 Lectures ( including this one!) still on the web at: http://www.le.ac.uk/physics/research/cmp/staff/bak.html Some (hopefully) useful points on semiconductors which you might (possibly) need to know …. Semiconductors Intrinsic semiconductors – pure, no impurities Extrinsic semiconductors – contain small amounts of deliberately added impurity (doped) Intrinsic Semiconductors Semiconducting elements e.g. Si, Ge (Group IV) - each atom bonded to 4 nearest neighbours i.e. tetrahedral bonding (2D – representation) Energy Band Diagram for Intrinsic Semiconductor (in real space) Energy, E Conduction Band (CB) Ec EF Energy Gap g Ev Valence Band (VB) Recall idea of energy bands for electrons in solids. energies of electrons lie in regions or bands. Bands separated by forbidden regions or energy gaps. Consider a material with either cimpletely filled or completely empty bands. T = 0 - Insulator T > 0 - some electrons from VB are excited into CB. Vacancies or “holes” are created in VB. For an intrinsic semiconductor nc= pv nc = electron conc’n in CB pv = hole conc’n in VB Both electrons in CB and (positive) holes in VB contribute to electrical conduction (in applied E-field) So for intrinsic semiconductor, electrical conductivity is given by: = ncee + pveh e – electron mobility h - hole mobility Definition of = (v/E) [v = carrier velocity in electric field E] Extrinsic (or Doped) Semiconductors n-type Doped Semiconductors These have small amounts of groupV impurities e.g. P, As e- bonds with neighbouring atoms 4 go to form bonds with neighbouring Si atoms P 5th electron is unpaired and weakly bound to P. Thermal excitation is usually enough to break bond between P and unpaired electron. e- This leaves an ionised P (donor atom) bonded to the Si network, and a free (donor) electron which can carry charge Donors can usually be considered to be completely ionised at room temperature. P+ Energy Band Diagram for n-type Semiconductor conduction band valence band EF Ec Ed Ev At T = 0, all donor electrons are weakly bound to P atoms. Represented on energy diagram by putting electrons in levels at Ed (donor levels) – just below Ec. Typically Ec – Ed = 0.01 – 0.1 eV This is small or comparable with thermal energies (kT = 0.025 eV at room temperature). So at room temperature, most of the donor atoms have given up their excess electron large increase in nc (concentration of electrons in conduction band) large increase in conductivity . So assuming all donors ionised, charge neutrality gives nc = pv + Nd [Nd = conc’n of donor atoms] which can normally approximate to nc ≈ Nd i.e. for n-type semiconductor, can normally neglect hole contribution Hence, for n-type at room temp, conductivity is ≈ ncee ≈ Ndee p-type Doped semiconductors Small amounts of Group III impurities e.g. B, Al B has 3 available electrons to form with neighbouring atoms. B adopts tetrahedral bonding but with broken bond. [In fact, broken bond shared between all 4 bonds to neighbouring Si’s] B Can regard as tetrahedrally bonded B binding a hole. B can capture (accept) an electron from a Si-Si bond elsewhere. This leaves a negatively ionised B atom (acceptor), and a broken Si-Si bond (mobile or free hole). B- Can think of B as donating a free hole. Process occurs easily at thermal energies (room temp’). Band diagram for p-type Semiconductor c F a v At T = 0, all B atoms have a weakly bound hole. Represented on energy diagram by putting holes on levels at Ea (acceptor levels) – just above Ev. Typically Ea – Ev = ~ 0.01 – 0.1 eV At room temperature, large numbers of electrons excited from VB into acceptor level a – leaves large number of holes in VB. [Alternatively: large numbers of holes excited down into VB - as in diagram] large increase in pv large increase inconductivity So assuming all acceptors ionised, charge neutrality gives pv = nc + Na [Na = acceptor conc’n] which can normally approximate to pv ≈ Na i.e. for p-type, can normally neglect electrons Hence, for p-type at room temp’, conductivity is ≈ pveh ≈ Naeh Temperature Dependence of nc and pv Important since this governs T-dependence of . Conc’n of electrons in conduction band, nc given by ( E EF ) nc = Nc exp c kT Nc - effective density of states at the conduction band edge. m kT Nc = 2 2 * 3 2 e 2 [me* - effective electron mass] Conc’n of holes in valence band, pv given by ( E EV ) pv = Nv exp F kT Nv - effective density of states at the valence band edge. m kT Nv = 2 2 * 3 2 h 2 [mh* - effective hole mass] Law of Mass Action Above expressions for nc and pv give for the product ncpv ( E Ev ) ncpv = NcNv exp c kT Since energy gap g = c - v E ncpv = NcNv exp g kT True for any semiconductor, whether intrinsic or doped. For an intrinsic semiconductor nc = pv = ni [ni - intrinsic carrier concentration] Hence Eg ncpv = ni = NcNv exp kT Law of Mass Action 2 3 2 m kT Nc = 2 and 2 * Using m kT Nv = 2 2 * e h 2 2 E ni = ( N c N v ) exp g 2kT 1 2 3 2 Eg kT ni = 2(me*m ) exp 2 2 2kT Exponential term dominates over kT term. 3 * 4 h 3 2 3 2 How do we obtain the expressions for nc and pv? Basic idea - integrate over all available energies in conduction band Conc’n of electrons between energy and + d is P()D()d P() is the Fermi-Dirac function 1 E EF 1 exp{ } kT [F = Fermi level; T = temperature] i.e. P() is the probability of occupation P() = D() is the density of states (per unit volume) in the conduction band. Assume D() is free-electronlike: i.e. D() = A( E Ec ) 1 2 *3 A= ( 2m ) 1 2 e 2 3 [me* - effective electron mass] Hence total conc’n of electrons in conduction band nc is nc = P()D()d c pv (hole conc’n in valence band) obtained in similar way Semiconductor Devices pn Junction Possible to fabricate wide range of devices by joining together different semiconductor types. One of the simplest of these - pn junction. Large number of devices based on this – lasers, solar cells, LEDs (remember the PBL??) Reminder of I-V behaviour of pn diode What happens when external bias (voltage) V is applied? How does I vary? What does it tell you? Operation of LED Band Diagrams ~ g zero bias c F v n p modest forward bias V eV large forward bias V eV large numbers of electrons flow from n to p (and holes from p to n) when eV > g Ideal I-V behaviour I = I0[exp(eV/kT) –1] - forward bias I = I0[1 – exp(-eV/kT)] - reverse bias N.B. - 2 carrier types. negative electrons flow from n to p positive holes flow in opposite direction. I V I0 So at large V, I predicted to increase ~ exponentially. In practice, I increases linearly with V for large V. Ohmic Region V g/e Once pn junction is forward biased by value greater than g/e, large numbers of electrons injected from n to p, and holes from p to n I becomes large and limited by series resistance of device. Ohmic behaviour is observed. [Could be due to contact resistance between metal and semiconductor, resistivity of the semiconductor, or series resistance of connecting wires]. Can extrapolate linear region back to I = 0 to obtain estimate for g (as done in PBL). LED (Light Emitting Diode) Emission Process Recombination of electron in conduction band with hole in valence band; energy released emitted as photon of well-defined frequency. For process to occur, semiconductor must have direct gap. E g g k Fig.1 ph k Fig.2 See original notes from Unit 4. Energy released in recombination event is g i.e. ph = g Both energy and momentum conserved ( k 0) LEDs make use of emission process in semiconductors. Consist of pn junction of a direct gap semiconductor, operated in forward bias. Basic operation 1. Electrons from n-region diffuse across depletion layer into narrow region just inside p-side. 2. Here, they recombine with holes, emitting photons. 3. Wavelength of light determined by energy gap g. Eg hc So could measure of emitted light by e.g. diffraction Could also use the I-V analysis